### van der Waals Interactions in Ionic and Semiconductor Solids

Guo-Xu Zhang, Alexandre Tkatchenko,*Joachim Paier, Heiko Appel, and Matthias Scheffler

Fritz-Haber-Institut der Max-Planck-Gesellschaft, Faradayweg 4-6, 14195, Berlin, Germany (Received 2 June 2011; published 5 December 2011)

van der Waals (vdW) energy corrected density-functional theory [Phys. Rev. Lett. 102, 073005 (2009)] is applied to study the cohesive properties of ionic and semiconductor solids (C, Si, Ge, GaAs, NaCl, and MgO). The required polarizability and dispersion coefficients are calculated using the dielectric function obtained from time-dependent density-functional theory. Coefficients for ‘‘atoms in the solid’’ are then calculated from the Hirshfeld partitioning of the electron density. It is shown that the Clausius-Mossotti equation that relates the polarizability and the dielectric function is accurate even for covalently-bonded semiconductors. We find an overall improvement in the cohesive properties of Si, Ge, GaAs, NaCl, and MgO, when vdW interactions are included on top of the Perdew-Burke-Ernzerhof or Heyd-Scuseria-Ernzerhof functionals. The relevance of our findings for other solids is discussed.

DOI:10.1103/PhysRevLett.107.245501 PACS numbers: 61.50.f, 71.10.w, 71.15.m

Cohesion in ionic and semiconductor solids arises mainly from electrostatic interactions and covalent bond-ing [1], and it is typically assumed that van der Waals (vdW) interactions play a minor role. Nevertheless, the qualitative and quantitative role of vdW interactions in solids has been a matter of discussion for quite some time [2–8]. Density-functional theory (DFT) is the method of choice for studying the bonding properties of solids. However, the widely used local-density approximation (LDA), generalized gradient approximation (GGA), as well as (screened) hybrid functionals are lacking the long-range vdW energy tail. Direct ab initio estimates of the vdW energy in solids have so far proven challenging. Recent many-body calculations using the random-phase approximation (RPA) [8–10], which includes the vdW energy seamlessly and accurately, yield significantly im-proved cohesive properties for a wide variety of solid-state systems over state-of-the-art (semi)-local DFT approxima-tions. However, the vdW energy can only be rigorously defined in the large-distance limit. The aim of this Letter is to calculate accurate atomic polarizabilities, vdW coeffi-cients, and vdW radii in ionic and semiconductor solids and to estimate the contribution of the long-range vdW energy to the cohesive properties. We find an overall improvement in the description of cohesion for model ionic and semiconductor solids when vdW interactions are in-cluded on top of the Perdew-Burke-Ernzerhof (PBE) [11] and the Heyd-Scuseria-Ernzerhof (HSE) [12,13] functionals.

The first step to calculate the vdW energy in a solid is to determine the frequency-dependent polarizability per

crystal unit cell. Two complementary schemes are fol-lowed in this work: (i) compute the polarizability per volume from the dielectric function of the solid, (ii) compute the polarizability per atom from cluster ex-trapolation. We find good agreement between these two different approaches, which justifies the concept of ‘‘atom in the solid.’’ The atomic polarizability in binary (or more complex) crystals is obtained from the Hirshfeld partition-ing of the electron density in a solid.

The frequency-dependent polarizability is related to the dielectric function as [14]

ð!Þ ¼ V "ð!Þ 1

L"ð!Þ L þ 4; (1) where ð!Þ is the polarizability per volume V at frequency !, "ð!Þ is the dielectric function of the solid, and L is the so-called Lorentz factor, which depends on the ionicity and hybridization [14]. The constant L is known for two limits: (i) electron gas, where L ¼ 0, (ii) ideal rare-gas solids and ideal ionic crystals, where L ¼ 4=3. In the latter case, Eq. (1) is known as the Clausius-Mossotti (CM) equation. In rare-gas and purely ionic crystals, the CM equation is an accurate approximation. However, the hybridization be-tween nearest neighbors in a covalently-bonded semicon-ductor is thought to lead to a significantly reduced value of the Lorentz factor [15].

An alternative and direct way to compute the polariz-ability in solids is through a cluster extrapolation (CE). For ionic crystals, the CE and CM procedures yield essentially the same result [16]. Thus, we concentrate here on showing that CE and CM also lead to very similar polarizabilities for semiconductor crystals. We illustrate our case for Si, however, the same conclusions can be made for C and Ge [17]. In the case of hydrogen-saturated semiconductor clusters, denoted as XiHj(X ¼ C, Si, or Ge; see Fig. 1),

there are four types of fourfold coordinated X atoms, the ‘‘bulklike’’ X atom, and surface X atoms bonded to one,

two, or 3 H atoms, respectively. For the XiHj cluster, the

total static polarizability is partitioned as

cluster ’ niXþ njH; (2)

where niand njare the numbers of X and H atoms of the

cluster, and X and H denote average static

polarizabil-ities. To obtain a converged bulk silicon atom polarizability Siand a dispersion coefficient CSiSi6 from the CE, we use a

set of 30 Si_{i}H_{j}clusters, from SiH_{4} to Si_{172}H_{120}, with the
geometries taken from Ref. [18]. We calculated the
frequency-dependent polarizability for every cluster at
the time-dependent density-functional level of theory
(TDLDA) using the same computational setup as in
Ref. [18]. To test the accuracy of the additivity
approxi-mation in Eq. (2), we perform a least-squares fit of Siand

H to a set of N ( 2) clusters, as shown in Fig.1. For

relatively small clusters, there are simply not enough bulk Si atoms, thus the obtained polarizabilities do not represent the crystal environment. However, for N 10 the fit con-verges to Si¼ 26:8 0:5 bohr3. Essentially the same

converged value (Si¼ 26:6 0:3 bohr3) is obtained

when starting from the largest cluster. These results indi-cate that the applied fitting procedure is robust. To obtain the bulk CSiSi

6 vdW coefficient, exactly the same procedure

was applied. In Fig.1 we also show the results of fitting CSiSi

6 on different clusters. The behavior of the fit is similar

to the case of static polarizability. We note that a similar procedure was recently used by Grimme et al. to determine atomic C6 coefficients from molecular TDDFT

calcula-tions [19].

In order to compare the CM and CE approaches, we carried out periodic and cluster TDDFT calculations for diamond, Si, and Ge as a function of the unit cell volume.

The computational details are reported in the supplemental material [17]. The bulk dielectric function was computed using both TDLDA and TDHSE with the so-called Nanoquanta (NQ) nonlocal exchange-correlation kernel [20], using the same approach as in Ref. [21]. When combined with TDHSE, the NQ kernel can correctly cap-ture excitonic effects, which are known to play an impor-tant role for the optical spectrum of semiconductors [22]. TDHSEþ NQ method yields excellent agreement for the static dielectric constant "1 with the experimental

refer-ence for ionic and semiconductor solids (see Table Iand Ref. [21]).

The comparison of CSiSi

6 of CM and CE is shown in

Fig. 2 as a function of the lattice constant. The static polarizability follows the same trend as C6. The

corre-sponding values at the equilibrium volume of C, Si, and Ge are given in the supplemental material [17]. For the range of investigated unit cell volumes, Si and CSiSi6

exhibit close to linear dependence on the lattice parameter. The maximum deviation between CM and CE is less than 0:5 bohr3 for Si (2%), and 9:0 hartree bohr6 for CSiSi6

(6%). Considering that both CM and CE rely on a number of approximations, the agreement between them is striking. It is noteworthy that the polarizability and C6 coefficients

in semiconductor crystals are significantly reduced com-pared to the free-atom values (CSiSi

6;free ¼ 305 hartree bohr6):

at the equilibrium volume, the C_{6}coefficient is reduced by
roughly a factor of 2. In fact, this finding holds for all solids
studied in this work, as can be seen in TableIby comparing
the C6 coefficients per unit cell with the respective

free-atom sum.

Seeking to understand the success of the CM equation
for a wide variety of solids, beyond ‘‘simple’’ rare-gas and
ideal ionic crystals, we use the DFTþ vdW method [24] to
calculate the C_{6}coefficients for atoms in semiconductors.
The DFTþ vdW method accurately takes into account the
short-range screening and hybridization contributions to
the polarizability. However, the long-range screening is

TABLE I. Calculated static dielectric constant "1 and C6
dispersion coefficients (in hartree bohr6 _{per unit cell) at the}
experimental lattice constants using the TDHSEþ NQ method
(fourth column—computed from the experimental dielectric
function). The experimental dielectric constants are taken from
Ref. [23]. The sixth column shows the sum of free-atom C6
coefficients per unit cell. The last two columns show partitioned
atomic C6 coefficients used for the vdW energy correction.

"Expt:1 "HSE1 CExpt:6cell CHSE6cell Cfree6cell Cð1Þð1Þ6atom Cð2Þð2Þ6atom

Cð1Þ 5.7 5.6 66.8 186 16.7 Sið1Þ 11.9 11.3 689 664 1220 166 Geð1Þ 16.0 15.9 898 1416 224 Mgð1ÞOð2Þ 3.0 2.8 56.3 59.3 797 38.6 2.2 Gað1ÞAsð2Þ 10.9 10.9 782 1398 213 179 Nað1ÞClð2Þ 2.3 2.3 174 2154 69.3 23.7

FIG. 1 (color online). Least-squares fitting results for the
po-larizability (top, in bohr3_{) and C}

neglected. For the Si crystal, the DFTþ vdW scheme yields Si¼ 35:0 bohr3 and CSiSi6 ¼ 280 hartree bohr6—

less than 10% decrease from the corresponding free-atom values. Thus, we conclude that the main factor for the polarizability reduction in solids is the long-range electro-static screening. In fact, Eq. (1) relates the dielectric func-tion to the atomic polarizability by including the collective electrostatic screening from all the dipoles in the crystal. For crystals with cubic symmetry (which holds for all solids studied in this work), this results in L ¼ 4=3, yielding the CM equation. The constant L is only modified due to short-range screening effects. Since we found the short-range screening to play a minor role for C, Si, Ge, and GaAs, this explains the success of the CM equation for semiconductors. The inclusion of screening effects beyond hybridization in the DFTþ vdW method is the subject of our current work [25].

The good agreement between the CM and CE
ap-proaches allows us to use either C_{6}ðVÞ values for
calculat-ing the vdW energy in solids. However, the best agreement
with the experimental reference is achieved with
TDHSEþ NQ calculations. In fact, when using the
experi-mental dielectric function of Si, the CSiSi

6 coefficient agrees

with the TDHSEþ NQ method to 3%. In the case of Ge,
the TDHSEþ NQ dielectric constant "_{1} is in excellent
agreement with measurements of Cardona et al. [26], thus
we use the polarizabilities and C6 coefficients from the

TDHSEþ NQ scheme for further discussion.

The missing long-range vdW energy is added to the DFT total energy on top of PBE [11] and HSE06 [13] func-tionals by using the DFTþ vdW approach [24]

EvdW¼ 1 2 X A;B fdðRAB; R0A; RB0ÞCAB6 R6AB; (3)

where RAB is the distance between atoms A and B, CAB6 is

the corresponding vdW coefficient, and R0Aand R0Bare the

vdW radii. The latter are defined as Rsolid vdW¼

ðsolid=freeÞ1=3RfreevdW, where RfreevdW is calculated as

de-scribed in Ref. [24]. The damping function fd cuts off

the interaction at short covalent distances. We use a Fermi-type damping function [27],

fdðRAB; R0ABÞ ¼ 1þ exp d RAB sRR0AB 11; (4) where R0AB¼ R0Aþ R0B, and d and sRare free parameters.

The sRparameter scales the vdW radius and is adjusted for

every DFT functional [28]. The d parameter controls the steepness of the damping function. For PBE we have determined sR¼ 0:94 and d ¼ 20 on a database of

accu-rate quantum-chemical calculations. For the HSE06 func-tional, sR ¼ 0:96 and d ¼ 20. The cohesive properties of

solids show little sensitivity to a reasonable variation of up to 5% for sR and 15% for d.

To extend the DFTþ vdW scheme to solids with several atomic elements per unit cell, we define AB¼ VAHirsh=VBHirsh, where VHirsh is the Hirshfeld

volume of an atom A or B in the solid [24]. Using the additivity ansatz for the polarizability, we obtain Bði!Þ ¼ solidði!Þ=ðABþ 1Þ and Aði!Þ ¼

solidði!ÞAB=ðABþ 1Þ, where solidði!Þ comes from

Eq. (1). With this definition the C_{6} coefficients (CAA
6 ,

CBB

6 , CAB6 ) can be obtained from the Casimir-Polder

inte-gral using Aði!Þ and Bði!Þ. This scheme can be easily

extended to ternary and more complex compounds by defining ACand so on. We have used the TDHSEþ NQ

dielectric function at the experimental lattice constant to compute solidði!Þ for GaAs, NaCl, and MgO.

Figure3summarizes the errors in the cohesive proper-ties obtained by using the Birch-Murnaghan equation of state [29] with standard and vdW-corrected PBE and HSE06 functionals for all solids studied in this work. The obtained values for every solid are shown in Tables IV and V of the supplemental material [17]. The zero-point energy (ZPE) within the harmonic approxima-tion is added to the ground-state energies at each volume for every functional. All DFT calculations, except HSE06, were done with the FHI-aims all-electron code [30], with LDA, PBE, and PBEsol cohesive properties in excellent agreement with WIEN2K [31]. The HSE06 calculations were done with the VASPcode [32], with ZPE correction

added using the PBE phonon spectra.

For the traditional functionals, the considered cohesive properties follow the well-known trend: the lattice con-stants with LDA are too small, the bulk moduli and cohe-sive energies are too large; PBE shows the opposite tendency, and PBEsol lies in between of LDA and PBE. The HSE06 method partially cures the self-interaction problem in LDA and GGA functionals, leading to signifi-cantly better electronic structure (e.g., band gaps and di-electric constants) of solids compared to LDA and GGA functionals [33]. For the same reason, the HSE06 method

also yields improved results for the lattice constants and bulk moduli of semiconductors and ionic solids. However, lattice constants are still somewhat overestimated, while the bulk moduli are underestimated in HSE06 calculations. Furthermore, the HSE06 scheme leads to underestimated cohesive energies (see supplemental material [17]), typi-cally very similar to the PBE functional. When the vdW energy is coupled with the PBE functional, the errors in all cohesive properties are reduced by a factor of 2 when compared to experimental data. The same improvement is found for the HSE06þ vdW method, except for the bulk moduli, where the errors remain roughly the same (under-estimation for HSE06 calculations, over(under-estimation for HSE06þ vdW calculations). It is well known that the optimal value of the range separation parameter in the HSE06 method depends on the electrostatic screening properties of the solid [13,33]. Hence, the improvement of bulk moduli in the HSE06þ vdW method requires further careful investigation.

For diamond, both the PBEþ vdW and the HSE06 þ vdW approaches yield slight overbinding. It is known, however, that anharmonic zero-point energy is important for diamond due to its relatively small mass, and will reduce the overbinding [34]. For Si and Ge, the vdW energy contributes 8% to the cohesive energy for both the PBEþ vdW and HSE06 þ vdW schemes, thus it can-not be considered negligible. The vdW energy also makes a visible contribution to the cohesive properties of GaAs, NaCl, and MgO. Both PBEþ vdW and HSE06 þ vdW results are in consistently better agreement with experi-ment than the standard functionals. The vdW energy con-tributes around 0:2 eV=atom to the cohesive energy for GaAs, NaCl, and MgO, and 9–16 GPa to the bulk modulus. The vdW concept is only cleanly defined at distances where the atomic electron densities do not overlap between

two atoms. For all values of sR and d in the damping

function [Eq. (4)] used in this work, the interaction be-tween the nearest neighbors in C, Si, and Ge crystals vanishes. The second-neighbor interaction is also damped depending on the sRparameter. For sR ¼ 1:0, the cohesive

energies and the bulk moduli change by less than a few percent, while the lattice constants are virtually unmodi-fied. Thus, we conclude that the obtained improvements with the PBEþ vdW and HSE06 þ vdW methods are due to the long-range vdW energy, and are not an artifact of the chosen damping function.

In summary, we obtained accurate vdW coefficients for atoms in ionic and semiconductor crystals using TDDFT calculations and the Clausius-Mossotti relation between the polarizability and the dielectric function. The DFTþ vdW method leads to overall improvement of the cohesive properties of ionic (NaCl, MgO) and semiconductor (Si, Ge, GaAs) solids. Despite the good agreement of the HSE06þ vdW method with experiment, there still re-mains room for improvement. For example, nonadditive many-body vdW energy is not accounted for in the HSE06þ vdW method. Also, anharmonic zero-point and temperature contributions to the cohesive properties should be included for the final comparison between experiment and theory. Note that it is well known that most GGA and hybrid functionals consistently underestimate cohesive en-ergies and bulk moduli, and overestimate lattice constants for a wide variety of semiconductors, ionic solids, and metals [35]. We thus conclude that our findings about the importance of the long-range vdW energy are likely to be valid beyond the benchmark semiconductors and ionic solids studied in this work.

A. T. acknowledges support from the European Research Council (ERC Starting Grant VDW-CMAT).

*tkatchen@fhi-berlin.mpg.de

[1] N. W. Ashcroft and N. D. Mermin, Solid State Physics (Holt, Reinhart & Winston, New York, 1976).

[2] J. E. Mayer,J. Chem. Phys. 1, 270 (1933).

[3] J. J. Rehr, E. Zaremba, and W. Kohn, Phys. Rev. B 12, 2062 (1975).

[4] D. D. Richardson and J. Mahanty, J. Phys. C 10, 3971 (1977).

[5] D. D. Richardson,J. Phys. C 11, 3779 (1978).

[6] J. Tao, J. P. Perdew, and A. Ruzsinszky,Phys. Rev. B 81, 233102 (2010).

[7] J. Klimesˇ, D. R. Bowler, and A. Michaelides,Phys. Rev. B 83, 195131 (2011).

[8] L. Romaner et al., Phys. Rev. Lett. (to be published). [9] J. Harl and G. Kresse, Phys. Rev. Lett. 103, 056401

(2009).

[10] J. Harl, L. Schimka, and G. Kresse, Phys. Rev. B 81, 115126 (2010).

[11] J. P. Perdew, K. Burke, and M. Ernzerhof,Phys. Rev. Lett. 77, 3865 (1996).

[12] J. Heyd, G. E. Scuseria, and M. Ernzerhof,J. Chem. Phys. 118, 8207 (2003).

[13] J. Heyd, G. E. Scuseria, and M. Ernzerhof,J. Chem. Phys. 124, 219906 (2006).

[14] J. R. Tessman, A. H. Kahn, and W. Shockley,Phys. Rev. 92, 890 (1953).

[15] N. F. Mott and R. W. Gurney, Electronic Processes in Ionic Crystals (Oxford University Press, London, 1948). [16] P. W. Fowler, P. J. Knowles, and N. C. Pyper,Mol. Phys.

56, 83 (1985).

[17] See Supplemental Material at http://link.aps.org/ supplemental/10.1103/PhysRevLett.107.245501 for com-putational details, polarizability, C6, and RvdW for all solids, along with experimental and calculated cohesive properties.

[18] S. Botti et al.,Phys. Rev. B 78, 035333 (2008).

[19] S. Grimme, J. Antony, S. Ehrlich, and H. Krieg,J. Chem. Phys. 132, 154104 (2010).

[20] A. Marini, R. Del Sole, and A. Rubio,Phys. Rev. Lett. 91, 256402 (2003).

[21] J. Paier, M. Marsman, and G. Kresse, Phys. Rev. B 78, 121201(R) (2008).

[22] S. Botti et al.,Phys. Rev. B 69, 155112 (2004). [23] J. A. Van Vechten,Phys. Rev. 182, 891 (1969).

[24] A. Tkatchenko and M. Scheffler, Phys. Rev. Lett. 102, 073005 (2009).

[25] A. Tkatchenko, R. A. DiStasio, Jr., R. Car, and M. Scheffler (unpublished).

[26] A. R. Gon˜i, K. Syassen, and M. Cardona,Phys. Rev. B 41, 10 104 (1990).

[27] Q. Wu and W. Yang,J. Chem. Phys. 116, 515 (2002). [28] P. Jurecˇka, J. Cˇ erny, P. Hobza, and D. R. Salahub, J.

Comput. Chem. 28, 555 (2007). [29] F. Birch,Phys. Rev. 71, 809 (1947).

[30] V. Blum et al.,Comput. Phys. Commun. 180, 2175 (2009). [31] P. Haas, F. Tran, and P. Blaha,Phys. Rev. B 79, 085104

(2009).

[32] G. Kresse and J. Furthmu¨ller,Comput. Mater. Sci. 6, 15 (1996).

[33] A. V. Krukau, O. A. Vydrov, A. F. Izmaylov, and G. E. Scuseria,J. Chem. Phys. 125, 224106 (2006).

[34] H. Jex,Phys. Status Solidi B 45, 343 (1971).

[35] L. Schimka, J. Harl, and G. Kresse,J. Chem. Phys. 134, 024116 (2011).

[36] V. N. Staroverov, G. E. Scuseria, J. Tao, and J. P. Perdew, Phys. Rev. B 69, 075102 (2004).